# Electronic Supplementary Material (ESI) for CrystEngComm.
# This journal is © The Royal Society of Chemistry 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_CP2019062906_0m
_database_code_depnum_ccdc_archive 'CCDC 2165495'
loop_
_audit_author_name
_audit_author_address
'Lubin Ni'
;Yangzhou University
China
;
_audit_update_record             
;
2022-09-05 deposited with the CCDC.	2022-10-12 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2017/1
_shelx_SHELXL_version_number     2017/1
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C60 Cu6 Mn0 Mo18 N12 O67 Si'
_chemical_formula_weight         4096.97

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 21/c'
_space_group_name_Hall           '-P 2ybc'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   13.9435(8)
_cell_length_b                   20.0147(12)
_cell_length_c                   17.2063(11)
_cell_angle_alpha                90
_cell_angle_beta                 93.972(2)
_cell_angle_gamma                90
_cell_volume                     4790.3(5)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    9854
_cell_measurement_theta_min      2.5507
_cell_measurement_theta_max      27.506

_exptl_crystal_description       bulk
_exptl_crystal_colour            colorless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.840
_exptl_crystal_F_000             3848
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.08
_exptl_absorpt_coefficient_mu    3.695
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.5372
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_process_details   
;
 SADABS 2016/2: Krause, L., Herbst-Irmer, R., Sheldrick G.M. & Stalke D.,
 J. Appl. Cryst. 48 (2015) 3-10
;
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  graphite
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            44626
_diffrn_reflns_av_unetI/netI     0.0414
_diffrn_reflns_av_R_equivalents  0.0486
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_theta_min         1.563
_diffrn_reflns_theta_max         27.103
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measured_fraction_theta_full 0.993
_diffrn_reflns_Laue_measured_fraction_max 0.992
_diffrn_reflns_Laue_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.992
_diffrn_reflns_point_group_measured_fraction_full 0.993
_reflns_number_total             10471
_reflns_number_gt                9192
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0462P)²+125.3760P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         10471
_refine_ls_number_parameters     739
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0766
_refine_ls_R_factor_gt           0.0674
_refine_ls_wR_factor_ref         0.1665
_refine_ls_wR_factor_gt          0.1617
_refine_ls_goodness_of_fit_ref   1.156
_refine_ls_restrained_S_all      1.156
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.35314(5) 0.58476(4) 0.95461(5) 0.01766(18) Uani 1 1 d . . . . .
Mo2 Mo 0.53381(6) 0.49588(4) 0.89839(5) 0.01701(17) Uani 1 1 d . . . . .
Mo3 Mo 0.35860(6) 0.40820(4) 0.96757(5) 0.01762(18) Uani 1 1 d . . . . .
Mo4 Mo 0.10660(9) 0.46585(5) 0.68767(6) 0.0375(3) Uani 1 1 d . . . . .
Mo5 Mo 0.25221(6) 0.50415(5) 0.53273(5) 0.0262(2) Uani 1 1 d . . . . .
Mo6 Mo 0.14623(7) 0.51246(5) 0.34067(6) 0.0293(2) Uani 1 1 d . . . . .
Mo7 Mo 0.12834(8) 0.34926(5) 0.53447(6) 0.0309(2) Uani 1 1 d . . . . .
Mo8 Mo -0.01122(7) 0.37481(5) 0.35684(7) 0.0345(2) Uani 1 1 d . . . . .
Mo9 Mo -0.12531(7) 0.35039(4) 0.53146(5) 0.0253(2) Uani 1 1 d . . . . .
Cu1 Cu 0.52262(9) 0.65906(6) 0.84874(7) 0.0231(3) Uani 1 1 d . . . . .
Cu2 Cu 0.53101(9) 0.32950(6) 0.86952(8) 0.0246(3) Uani 1 1 d . . . . .
Cu3 Cu 0.14260(8) 0.49076(6) 0.90612(7) 0.0214(3) Uani 1 1 d . . . . .
Si1 Si 0.000000 0.500000 0.500000 0.0179(7) Uani 1 2 d S . P . .
O1 O -0.1896(8) 0.2811(4) 0.5419(6) 0.052(3) Uani 1 1 d . . . . .
O15A O 0.0898(10) 0.3211(8) 0.4314(8) 0.021(3) Uiso 0.5 1 d . . P A 2
O15B O 0.0931(10) 0.3577(8) 0.4358(8) 0.025(3) Uiso 0.5 1 d . . P A 1
O2 O -0.1444(9) 0.3945(5) 0.6218(5) 0.064(3) Uani 1 1 d . . . . .
O3 O -0.0971(10) 0.4687(7) 0.5279(8) 0.080(4) Uani 1 1 d . . . . .
O4 O -0.0045(7) 0.3214(8) 0.5587(6) 0.083(5) Uani 1 1 d . . . . .
O5 O -0.0978(7) 0.3403(8) 0.4208(5) 0.077(4) Uani 1 1 d . . . . .
O6 O -0.0173(7) 0.4566(5) 0.7094(11) 0.105(6) Uani 1 1 d . . . . .
O7 O -0.0069(10) 0.5152(7) 0.5957(8) 0.081(4) Uani 1 1 d . . . . .
O8 O 0.1626(6) 0.4579(5) 0.7756(5) 0.043(2) Uani 1 1 d . . . . .
O9 O 0.1232(10) 0.3860(6) 0.6431(6) 0.083(5) Uani 1 1 d . . . . .
O10 O 0.0949(9) 0.4663(8) 0.5471(8) 0.082(4) Uani 1 1 d . . . . .
O11 O -0.0022(10) 0.4189(7) 0.4877(8) 0.081(4) Uani 1 1 d . . . . .
O12 O -0.0883(8) 0.4338(6) 0.3047(11) 0.106(6) Uani 1 1 d . . . . .
O13 O -0.0046(6) 0.3140(5) 0.2919(5) 0.043(2) Uani 1 1 d . . . . .
O14 O 0.1002(7) 0.4283(5) 0.3276(12) 0.115(7) Uani 1 1 d . . . . .
O16 O 0.2089(8) 0.5228(5) 0.2636(5) 0.048(2) Uani 1 1 d . . . . .
O17 O 0.2371(10) 0.4940(5) 0.4167(5) 0.070(4) Uani 1 1 d . . . . .
O18 O 0.3704(6) 0.4991(5) 0.5412(7) 0.062(3) Uani 1 1 d . . . . .
O19 O 0.2258(12) 0.4065(6) 0.5222(7) 0.095(6) Uani 1 1 d . . . . .
O20 O 0.2203(12) 0.4994(5) 0.6324(7) 0.093(5) Uani 1 1 d . . . . .
O21 O 0.2310(9) 0.5926(5) 0.5186(5) 0.062(3) Uani 1 1 d . . . . .
O22 O 0.2382(5) 0.4230(4) 0.9349(4) 0.0248(15) Uani 1 1 d . . . . .
O23 O 0.2343(5) 0.5628(4) 0.9208(4) 0.0247(15) Uani 1 1 d . . . . .
O24 O 0.3436(5) 0.6422(4) 1.0286(5) 0.0303(17) Uani 1 1 d . . . . .
O25 O 0.3976(5) 0.6327(3) 0.8783(4) 0.0259(15) Uani 1 1 d . . . . .
O26 O 0.5534(5) 0.5632(3) 0.8366(4) 0.0218(14) Uani 1 1 d . . . . .
O27 O 0.6490(5) 0.5002(3) 0.9657(4) 0.0190(13) Uani 1 1 d . . . . .
O28 O 0.4002(5) 0.4939(3) 0.8939(4) 0.0181(13) Uani 1 1 d . . . . .
O29 O 0.5021(4) 0.4359(3) 1.0046(4) 0.0174(13) Uani 1 1 d . . . . .
O30 O 0.5581(5) 0.4239(3) 0.8459(4) 0.0231(14) Uani 1 1 d . . . . .
O31 O 0.4051(5) 0.3555(4) 0.8962(4) 0.0264(16) Uani 1 1 d . . . . .
O32 O 0.3546(5) 0.3561(4) 1.0466(4) 0.0256(15) Uani 1 1 d . . . . .
O33 O 0.1856(7) 0.2785(5) 0.5571(7) 0.060(3) Uani 1 1 d . . . . .
N1 N 0.0329(6) 0.5541(5) 0.8928(5) 0.0239(18) Uani 1 1 d . . . . .
N2 N 0.0354(6) 0.4259(5) 0.9102(5) 0.0243(18) Uani 1 1 d . . . . .
N3 N 0.6257(6) 0.6944(5) 0.7867(5) 0.031(2) Uani 1 1 d . . . . .
N4 N 0.4961(7) 0.7554(4) 0.8631(5) 0.0272(19) Uani 1 1 d . . . . .
N5 N 0.6346(6) 0.2894(4) 0.8128(5) 0.0274(19) Uani 1 1 d . . . . .
N6 N 0.5040(7) 0.2355(5) 0.8916(6) 0.034(2) Uani 1 1 d . . . . .
C1 C 0.4229(8) 0.7798(7) 0.9007(8) 0.039(3) Uani 1 1 d . . . . .
C2 C 0.4099(11) 0.8485(7) 0.9066(11) 0.062(5) Uani 1 1 d . . . . .
C3 C 0.4744(16) 0.8911(8) 0.8745(14) 0.084(6) Uani 1 1 d . . . . .
C4 C 0.5492(12) 0.8649(7) 0.8350(11) 0.061(4) Uani 1 1 d . . . . .
C5 C 0.5589(8) 0.7957(5) 0.8299(7) 0.030(2) Uani 1 1 d . . . . .
C6 C 0.6338(8) 0.7624(6) 0.7884(6) 0.030(2) Uani 1 1 d . . . . .
C7 C 0.7073(10) 0.7946(9) 0.7531(8) 0.053(4) Uani 1 1 d . . . . .
C8 C 0.7718(12) 0.7577(10) 0.7156(9) 0.066(5) Uani 1 1 d . . . . .
C9 C 0.7613(11) 0.6900(10) 0.7104(11) 0.068(5) Uani 1 1 d . . . . .
C10 C 0.6847(10) 0.6567(8) 0.7478(8) 0.049(4) Uani 1 1 d . . . . .
C11 C 0.6998(9) 0.3223(7) 0.7762(7) 0.037(3) Uani 1 1 d . . . . .
C12 C 0.7756(10) 0.2874(9) 0.7412(8) 0.053(4) Uani 1 1 d . . . . .
C13 C 0.7786(12) 0.2207(9) 0.7460(9) 0.060(5) Uani 1 1 d . . . . .
C14 C 0.7098(12) 0.1849(8) 0.7844(8) 0.053(4) Uani 1 1 d . . . . .
C15 C 0.6382(9) 0.2218(6) 0.8170(7) 0.032(2) Uani 1 1 d . . . . .
C16 C 0.4295(9) 0.2153(6) 0.9340(9) 0.046(3) Uani 1 1 d . . . . .
C17 C 0.4101(13) 0.1467(8) 0.9426(13) 0.072(5) Uani 1 1 d . . . . .
C18 C 0.4688(14) 0.1020(8) 0.9083(14) 0.081(6) Uani 1 1 d . . . . .
C19 C 0.5473(12) 0.1223(7) 0.8655(11) 0.059(4) Uani 1 1 d . . . . .
C20 C 0.5605(9) 0.1909(5) 0.8584(8) 0.036(3) Uani 1 1 d . . . . .
C21 C 0.0480(9) 0.3595(6) 0.9195(7) 0.035(3) Uani 1 1 d . . . . .
C22 C -0.0311(8) 0.3167(6) 0.9229(8) 0.038(3) Uani 1 1 d . . . . .
C23 C -0.1250(8) 0.3448(7) 0.9173(7) 0.038(3) Uani 1 1 d . . . . .
C24 C -0.1346(7) 0.4134(6) 0.9068(6) 0.028(2) Uani 1 1 d . . . . .
C25 C -0.0536(7) 0.4527(6) 0.9033(5) 0.025(2) Uani 1 1 d . . . . .
C26 C -0.0554(7) 0.5248(6) 0.8942(6) 0.026(2) Uani 1 1 d . . . . .
C27 C -0.1389(7) 0.5623(7) 0.8912(6) 0.033(3) Uani 1 1 d . . . . .
C28 C -0.1305(8) 0.6328(7) 0.8856(7) 0.036(3) Uani 1 1 d . . . . .
C29 C -0.0415(9) 0.6616(7) 0.8818(7) 0.038(3) Uani 1 1 d . . . . .
C30 C 0.0396(8) 0.6206(6) 0.8866(7) 0.029(2) Uani 1 1 d . . . . .
O34 O 0.3671(19) 0.5056(13) 0.7306(15) 0.073(7) Uiso 0.5 1 d . . P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O24 1.728(8) . ?
Mo1 O25 1.772(7) . ?
Mo1 O23 1.773(7) . ?
Mo1 O29 2.131(6) 3_667 ?
Mo1 O27 2.186(7) 3_667 ?
Mo1 O28 2.219(7) . ?
Mo2 O30 1.747(7) . ?
Mo2 O26 1.749(7) . ?
Mo2 O28 1.860(7) . ?
Mo2 O27 1.915(6) . ?
Mo2 O29 2.240(7) 3_667 ?
Mo2 O29 2.256(6) . ?
Mo3 O32 1.717(7) . ?
Mo3 O22 1.758(7) . ?
Mo3 O31 1.775(7) . ?
Mo3 O29 2.130(6) . ?
Mo3 O27 2.170(6) 3_667 ?
Mo3 O28 2.234(6) . ?
Mo4 O8 1.662(8) . ?
Mo4 O9 1.794(11) . ?
Mo4 O6 1.802(13) . ?
Mo4 O20 2.020(12) . ?
Mo4 O12 2.031(12) 3_566 ?
Mo4 O7 2.374(14) . ?
Mo4 O10 2.413(14) . ?
Mo5 O18 1.647(9) . ?
Mo5 O20 1.803(10) . ?
Mo5 O21 1.808(9) . ?
Mo5 O19 1.995(10) . ?
Mo5 O17 2.004(9) . ?
Mo5 O10 2.350(13) . ?
Mo5 O3 2.397(15) 3_566 ?
Mo6 O16 1.650(8) . ?
Mo6 O17 1.795(11) . ?
Mo6 O14 1.810(11) . ?
Mo6 O2 1.971(9) 3_566 ?
Mo6 O6 2.036(10) 3_566 ?
Mo6 O7 2.361(13) 3_566 ?
Mo6 O3 2.438(13) 3_566 ?
Mo7 O33 1.659(8) . ?
Mo7 O15B 1.743(14) . ?
Mo7 O19 1.801(11) . ?
Mo7 O15A 1.903(13) . ?
Mo7 O4 2.006(11) . ?
Mo7 O9 2.015(10) . ?
Mo7 O11 2.387(13) . ?
Mo7 O10 2.402(15) . ?
Mo8 O13 1.659(8) . ?
Mo8 O12 1.794(11) . ?
Mo8 O5 1.825(11) . ?
Mo8 O15B 1.950(14) . ?
Mo8 O14 1.981(11) . ?
Mo8 O15A 2.129(14) . ?
Mo8 O7 2.356(14) 3_566 ?
Mo8 O11 2.413(14) . ?
Mo9 O1 1.667(9) . ?
Mo9 O4 1.812(10) . ?
Mo9 O2 1.823(9) . ?
Mo9 O5 1.978(9) . ?
Mo9 O21 2.010(9) 3_566 ?
Mo9 O11 2.360(14) . ?
Mo9 O3 2.401(13) . ?
Cu1 O25 1.924(7) . ?
Cu1 N3 1.979(9) . ?
Cu1 O26 1.980(7) . ?
Cu1 N4 1.983(9) . ?
Cu1 O32 2.417(7) 3_667 ?
Cu2 O31 1.917(7) . ?
Cu2 N6 1.960(9) . ?
Cu2 N5 1.970(9) . ?
Cu2 O30 1.974(7) . ?
Cu3 O23 1.932(7) . ?
Cu3 O22 1.942(7) . ?
Cu3 N2 1.985(8) . ?
Cu3 N1 1.988(9) . ?
Cu3 O8 2.375(9) . ?
Si1 O3 1.596(14) 3_566 ?
Si1 O3 1.596(14) . ?
Si1 O11 1.638(14) . ?
Si1 O11 1.638(14) 3_566 ?
Si1 O10 1.647(14) . ?
Si1 O10 1.647(14) 3_566 ?
Si1 O7 1.684(14) . ?
Si1 O7 1.684(14) 3_566 ?
N1 C30 1.340(14) . ?
N1 C26 1.365(13) . ?
N2 C21 1.348(15) . ?
N2 C25 1.350(13) . ?
N3 C10 1.331(17) . ?
N3 C6 1.366(15) . ?
N4 C1 1.337(15) . ?
N4 C5 1.347(14) . ?
N5 C11 1.318(15) . ?
N5 C15 1.354(14) . ?
N6 C20 1.344(16) . ?
N6 C16 1.372(16) . ?
C1 C2 1.391(18) . ?
C2 C3 1.38(3) . ?
C3 C4 1.39(3) . ?
C4 C5 1.394(18) . ?
C5 C6 1.466(17) . ?
C6 C7 1.386(16) . ?
C7 C8 1.36(3) . ?
C8 C9 1.37(3) . ?
C9 C10 1.446(19) . ?
C11 C12 1.434(18) . ?
C12 C13 1.34(2) . ?
C13 C14 1.40(3) . ?
C14 C15 1.390(18) . ?
C15 C20 1.474(18) . ?
C16 C17 1.409(19) . ?
C17 C18 1.37(3) . ?
C18 C19 1.42(3) . ?
C19 C20 1.392(17) . ?
C21 C22 1.401(16) . ?
C22 C23 1.423(18) . ?
C23 C24 1.389(18) . ?
C24 C25 1.381(15) . ?
C25 C26 1.452(16) . ?
C26 C27 1.383(15) . ?
C27 C28 1.419(19) . ?
C28 C29 1.374(18) . ?
C29 C30 1.395(16) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O24 Mo1 O25 103.5(4) . . ?
O24 Mo1 O23 106.8(3) . . ?
O25 Mo1 O23 105.0(3) . . ?
O24 Mo1 O29 90.3(3) . 3_667 ?
O25 Mo1 O29 88.7(3) . 3_667 ?
O23 Mo1 O29 154.5(3) . 3_667 ?
O24 Mo1 O27 92.9(3) . 3_667 ?
O25 Mo1 O27 155.0(3) . 3_667 ?
O23 Mo1 O27 87.7(3) . 3_667 ?
O29 Mo1 O27 72.3(2) 3_667 3_667 ?
O24 Mo1 O28 158.9(3) . . ?
O25 Mo1 O28 88.0(3) . . ?
O23 Mo1 O28 86.7(3) . . ?
O29 Mo1 O28 72.1(2) 3_667 . ?
O27 Mo1 O28 71.1(2) 3_667 . ?
O30 Mo2 O26 106.1(3) . . ?
O30 Mo2 O28 101.0(3) . . ?
O26 Mo2 O28 100.9(3) . . ?
O30 Mo2 O27 99.5(3) . . ?
O26 Mo2 O27 100.0(3) . . ?
O28 Mo2 O27 145.3(3) . . ?
O30 Mo2 O29 161.8(3) . 3_667 ?
O26 Mo2 O29 92.0(3) . 3_667 ?
O28 Mo2 O29 76.7(3) . 3_667 ?
O27 Mo2 O29 75.1(3) . 3_667 ?
O30 Mo2 O29 92.0(3) . . ?
O26 Mo2 O29 161.8(3) . . ?
O28 Mo2 O29 76.7(3) . . ?
O27 Mo2 O29 74.8(3) . . ?
O29 Mo2 O29 69.8(3) 3_667 . ?
O32 Mo3 O22 105.8(3) . . ?
O32 Mo3 O31 102.7(4) . . ?
O22 Mo3 O31 105.4(3) . . ?
O32 Mo3 O29 90.1(3) . . ?
O22 Mo3 O29 155.2(3) . . ?
O31 Mo3 O29 88.9(3) . . ?
O32 Mo3 O27 95.1(3) . 3_667 ?
O22 Mo3 O27 86.9(3) . 3_667 ?
O31 Mo3 O27 154.4(3) . 3_667 ?
O29 Mo3 O27 72.6(2) . 3_667 ?
O32 Mo3 O28 160.0(3) . . ?
O22 Mo3 O28 88.2(3) . . ?
O31 Mo3 O28 86.7(3) . . ?
O29 Mo3 O28 72.2(2) . . ?
O27 Mo3 O28 71.1(2) 3_667 . ?
O8 Mo4 O9 103.7(6) . . ?
O8 Mo4 O6 101.4(7) . . ?
O9 Mo4 O6 98.7(6) . . ?
O8 Mo4 O20 97.3(6) . . ?
O9 Mo4 O20 88.0(4) . . ?
O6 Mo4 O20 158.0(7) . . ?
O8 Mo4 O12 95.1(6) . 3_566 ?
O9 Mo4 O12 158.4(7) . 3_566 ?
O6 Mo4 O12 87.8(5) . 3_566 ?
O20 Mo4 O12 79.0(6) . 3_566 ?
O8 Mo4 O7 153.7(5) . . ?
O9 Mo4 O7 100.7(6) . . ?
O6 Mo4 O7 65.0(6) . . ?
O20 Mo4 O7 93.2(6) . . ?
O12 Mo4 O7 63.3(5) 3_566 . ?
O8 Mo4 O10 155.3(5) . . ?
O9 Mo4 O10 65.0(5) . . ?
O6 Mo4 O10 102.1(7) . . ?
O20 Mo4 O10 61.8(5) . . ?
O12 Mo4 O10 93.5(7) 3_566 . ?
O7 Mo4 O10 48.3(5) . . ?
O18 Mo5 O20 102.9(7) . . ?
O18 Mo5 O21 103.0(6) . . ?
O20 Mo5 O21 97.5(5) . . ?
O18 Mo5 O19 97.2(6) . . ?
O20 Mo5 O19 88.7(4) . . ?
O21 Mo5 O19 156.9(7) . . ?
O18 Mo5 O17 96.7(6) . . ?
O20 Mo5 O17 157.9(7) . . ?
O21 Mo5 O17 87.7(4) . . ?
O19 Mo5 O17 78.7(5) . . ?
O18 Mo5 O10 155.0(6) . . ?
O20 Mo5 O10 65.8(6) . . ?
O21 Mo5 O10 100.6(6) . . ?
O19 Mo5 O10 61.7(6) . . ?
O17 Mo5 O10 92.2(6) . . ?
O18 Mo5 O3 156.8(6) . 3_566 ?
O20 Mo5 O3 98.7(7) . 3_566 ?
O21 Mo5 O3 65.5(5) . 3_566 ?
O19 Mo5 O3 91.6(6) . 3_566 ?
O17 Mo5 O3 63.9(5) . 3_566 ?
O10 Mo5 O3 45.4(5) . 3_566 ?
O16 Mo6 O17 103.0(6) . . ?
O16 Mo6 O14 102.7(7) . . ?
O17 Mo6 O14 97.2(6) . . ?
O16 Mo6 O2 99.5(5) . 3_566 ?
O17 Mo6 O2 88.8(4) . 3_566 ?
O14 Mo6 O2 155.0(7) . 3_566 ?
O16 Mo6 O6 97.1(6) . 3_566 ?
O17 Mo6 O6 158.3(7) . 3_566 ?
O14 Mo6 O6 86.3(4) . 3_566 ?
O2 Mo6 O6 79.6(5) 3_566 3_566 ?
O16 Mo6 O7 154.2(5) . 3_566 ?
O17 Mo6 O7 100.1(6) . 3_566 ?
O14 Mo6 O7 62.9(6) . 3_566 ?
O2 Mo6 O7 92.3(5) 3_566 3_566 ?
O6 Mo6 O7 62.4(6) 3_566 3_566 ?
O16 Mo6 O3 157.6(5) . 3_566 ?
O17 Mo6 O3 65.5(5) . 3_566 ?
O14 Mo6 O3 98.0(7) . 3_566 ?
O2 Mo6 O3 62.5(5) 3_566 3_566 ?
O6 Mo6 O3 92.8(6) 3_566 3_566 ?
O7 Mo6 O3 46.6(5) 3_566 3_566 ?
O33 Mo7 O15B 114.2(7) . . ?
O33 Mo7 O19 102.5(7) . . ?
O15B Mo7 O19 89.4(7) . . ?
O33 Mo7 O15A 93.8(6) . . ?
O19 Mo7 O15A 104.3(6) . . ?
O33 Mo7 O4 98.6(6) . . ?
O15B Mo7 O4 91.6(6) . . ?
O19 Mo7 O4 156.4(7) . . ?
O15A Mo7 O4 84.6(5) . . ?
O33 Mo7 O9 98.1(6) . . ?
O15B Mo7 O9 147.4(7) . . ?
O19 Mo7 O9 87.2(4) . . ?
O15A Mo7 O9 161.3(6) . . ?
O4 Mo7 O9 79.4(5) . . ?
O33 Mo7 O11 157.0(5) . . ?
O15B Mo7 O11 57.2(6) . . ?
O19 Mo7 O11 98.8(7) . . ?
O15A Mo7 O11 72.5(5) . . ?
O4 Mo7 O11 62.5(5) . . ?
O9 Mo7 O11 91.4(6) . . ?
O33 Mo7 O10 154.8(6) . . ?
O15B Mo7 O10 87.1(6) . . ?
O19 Mo7 O10 62.8(6) . . ?
O15A Mo7 O10 109.2(6) . . ?
O4 Mo7 O10 93.7(6) . . ?
O9 Mo7 O10 62.6(5) . . ?
O11 Mo7 O10 46.6(5) . . ?
O13 Mo8 O12 101.8(7) . . ?
O13 Mo8 O5 101.5(6) . . ?
O12 Mo8 O5 98.8(6) . . ?
O13 Mo8 O15B 105.5(6) . . ?
O12 Mo8 O15B 148.8(7) . . ?
O5 Mo8 O15B 90.3(5) . . ?
O13 Mo8 O14 98.3(6) . . ?
O12 Mo8 O14 88.3(5) . . ?
O5 Mo8 O14 157.1(7) . . ?
O15B Mo8 O14 73.2(6) . . ?
O13 Mo8 O15A 88.3(5) . . ?
O12 Mo8 O15A 169.0(6) . . ?
O5 Mo8 O15A 83.3(5) . . ?
O14 Mo8 O15A 85.9(5) . . ?
O13 Mo8 O7 155.4(5) . 3_566 ?
O12 Mo8 O7 66.7(6) . 3_566 ?
O5 Mo8 O7 101.8(6) . 3_566 ?
O15B Mo8 O7 82.3(6) . 3_566 ?
O14 Mo8 O7 61.0(6) . 3_566 ?
O13 Mo8 O11 153.5(5) . . ?
O12 Mo8 O11 102.5(7) . . ?
O5 Mo8 O11 64.5(5) . . ?
O15B Mo8 O11 55.0(5) . . ?
O14 Mo8 O11 92.8(7) . . ?
O15A Mo8 O11 68.5(5) . . ?
O7 Mo8 O11 48.5(5) 3_566 . ?
O1 Mo9 O4 101.7(6) . . ?
O1 Mo9 O2 101.5(6) . . ?
O4 Mo9 O2 97.0(5) . . ?
O1 Mo9 O5 99.2(6) . . ?
O4 Mo9 O5 88.7(4) . . ?
O2 Mo9 O5 156.8(6) . . ?
O1 Mo9 O21 97.7(5) . 3_566 ?
O4 Mo9 O21 159.0(6) . 3_566 ?
O2 Mo9 O21 86.8(4) . 3_566 ?
O5 Mo9 O21 80.3(4) . 3_566 ?
O1 Mo9 O11 157.8(5) . . ?
O4 Mo9 O11 65.5(6) . . ?
O2 Mo9 O11 98.2(6) . . ?
O5 Mo9 O11 63.8(5) . . ?
O21 Mo9 O11 93.5(5) 3_566 . ?
O1 Mo9 O3 155.9(5) . . ?
O4 Mo9 O3 99.9(6) . . ?
O2 Mo9 O3 65.0(5) . . ?
O5 Mo9 O3 91.9(6) . . ?
O21 Mo9 O3 63.0(5) 3_566 . ?
O11 Mo9 O3 45.2(5) . . ?
O25 Cu1 N3 161.1(3) . . ?
O25 Cu1 O26 88.2(3) . . ?
N3 Cu1 O26 96.8(4) . . ?
O25 Cu1 N4 93.0(3) . . ?
N3 Cu1 N4 82.4(4) . . ?
O26 Cu1 N4 178.0(3) . . ?
O25 Cu1 O32 112.1(3) . 3_667 ?
N3 Cu1 O32 86.7(3) . 3_667 ?
O26 Cu1 O32 79.0(3) . 3_667 ?
N4 Cu1 O32 99.1(3) . 3_667 ?
O31 Cu2 N6 91.3(4) . . ?
O31 Cu2 N5 160.8(3) . . ?
N6 Cu2 N5 82.1(4) . . ?
O31 Cu2 O30 88.9(3) . . ?
N6 Cu2 O30 179.3(4) . . ?
N5 Cu2 O30 97.5(3) . . ?
O23 Cu3 O22 92.9(3) . . ?
O23 Cu3 N2 167.6(3) . . ?
O22 Cu3 N2 92.3(3) . . ?
O23 Cu3 N1 92.1(3) . . ?
O22 Cu3 N1 169.8(3) . . ?
N2 Cu3 N1 81.1(4) . . ?
O23 Cu3 O8 102.2(3) . . ?
O22 Cu3 O8 85.6(3) . . ?
N2 Cu3 O8 89.4(3) . . ?
N1 Cu3 O8 102.0(3) . . ?
O3 Si1 O3 180.0 3_566 . ?
O3 Si1 O11 111.1(7) 3_566 . ?
O3 Si1 O11 68.9(7) . . ?
O3 Si1 O11 68.9(7) 3_566 3_566 ?
O3 Si1 O11 111.1(7) . 3_566 ?
O11 Si1 O11 180.0(9) . 3_566 ?
O3 Si1 O10 68.9(7) 3_566 . ?
O3 Si1 O10 111.1(7) . . ?
O11 Si1 O10 70.4(7) . . ?
O11 Si1 O10 109.6(7) 3_566 . ?
O3 Si1 O10 111.1(7) 3_566 3_566 ?
O3 Si1 O10 68.9(7) . 3_566 ?
O11 Si1 O10 109.6(7) . 3_566 ?
O11 Si1 O10 70.4(7) 3_566 3_566 ?
O10 Si1 O10 180.0 . 3_566 ?
O3 Si1 O7 109.3(7) 3_566 . ?
O3 Si1 O7 70.7(7) . . ?
O11 Si1 O7 107.7(7) . . ?
O11 Si1 O7 72.3(7) 3_566 . ?
O10 Si1 O7 72.0(7) . . ?
O10 Si1 O7 108.0(7) 3_566 . ?
O3 Si1 O7 70.7(7) 3_566 3_566 ?
O3 Si1 O7 109.3(7) . 3_566 ?
O11 Si1 O7 72.3(7) . 3_566 ?
O11 Si1 O7 107.7(7) 3_566 3_566 ?
O10 Si1 O7 108.0(7) . 3_566 ?
O10 Si1 O7 72.0(7) 3_566 3_566 ?
O7 Si1 O7 180.0 . 3_566 ?
Mo7 O15A Mo8 123.0(7) . . ?
Mo7 O15B Mo8 147.4(9) . . ?
Mo9 O2 Mo6 138.0(6) . 3_566 ?
Si1 O3 Mo5 122.6(7) . 3_566 ?
Si1 O3 Mo9 122.6(7) . . ?
Mo5 O3 Mo9 95.2(5) 3_566 . ?
Si1 O3 Mo6 121.1(7) . 3_566 ?
Mo5 O3 Mo6 93.8(5) 3_566 3_566 ?
Mo9 O3 Mo6 94.1(5) . 3_566 ?
Mo9 O4 Mo7 135.5(8) . . ?
Mo8 O5 Mo9 136.2(8) . . ?
Mo4 O6 Mo6 135.4(9) . 3_566 ?
Si1 O7 Mo8 119.7(7) . 3_566 ?
Si1 O7 Mo6 121.0(8) . 3_566 ?
Mo8 O7 Mo6 97.5(5) 3_566 3_566 ?
Si1 O7 Mo4 119.8(7) . . ?
Mo8 O7 Mo4 96.2(5) 3_566 . ?
Mo6 O7 Mo4 97.2(5) 3_566 . ?
Mo4 O8 Cu3 139.1(5) . . ?
Mo4 O9 Mo7 137.3(8) . . ?
Si1 O10 Mo5 122.7(8) . . ?
Si1 O10 Mo7 120.6(7) . . ?
Mo5 O10 Mo7 96.7(5) . . ?
Si1 O10 Mo4 119.4(7) . . ?
Mo5 O10 Mo4 96.2(5) . . ?
Mo7 O10 Mo4 95.0(5) . . ?
Si1 O11 Mo9 122.8(7) . . ?
Si1 O11 Mo7 121.9(7) . . ?
Mo9 O11 Mo7 96.2(5) . . ?
Si1 O11 Mo8 118.8(7) . . ?
Mo9 O11 Mo8 95.4(5) . . ?
Mo7 O11 Mo8 95.2(5) . . ?
Mo8 O12 Mo4 133.8(9) . 3_566 ?
Mo6 O14 Mo8 138.5(10) . . ?
Mo6 O17 Mo5 136.5(7) . . ?
Mo7 O19 Mo5 138.5(9) . . ?
Mo5 O20 Mo4 136.0(8) . . ?
Mo5 O21 Mo9 136.2(7) . 3_566 ?
Mo3 O22 Cu3 145.3(4) . . ?
Mo1 O23 Cu3 145.4(4) . . ?
Mo1 O25 Cu1 135.6(4) . . ?
Mo2 O26 Cu1 129.7(4) . . ?
Mo2 O27 Mo3 106.8(3) . 3_667 ?
Mo2 O27 Mo1 107.3(3) . 3_667 ?
Mo3 O27 Mo1 108.8(3) 3_667 3_667 ?
Mo2 O28 Mo1 106.9(3) . . ?
Mo2 O28 Mo3 106.9(3) . . ?
Mo1 O28 Mo3 105.4(3) . . ?
Mo3 O29 Mo1 153.7(3) . 3_667 ?
Mo3 O29 Mo2 97.3(3) . 3_667 ?
Mo1 O29 Mo2 97.4(2) 3_667 3_667 ?
Mo3 O29 Mo2 97.4(2) . . ?
Mo1 O29 Mo2 97.8(3) 3_667 . ?
Mo2 O29 Mo2 110.2(3) 3_667 . ?
Mo2 O30 Cu2 129.5(4) . . ?
Mo3 O31 Cu2 135.3(4) . . ?
Mo3 O32 Cu1 127.3(4) . 3_667 ?
C30 N1 C26 119.8(10) . . ?
C30 N1 Cu3 125.8(7) . . ?
C26 N1 Cu3 114.3(7) . . ?
C21 N2 C25 120.9(9) . . ?
C21 N2 Cu3 123.8(7) . . ?
C25 N2 Cu3 115.3(7) . . ?
C10 N3 C6 121.5(11) . . ?
C10 N3 Cu1 124.4(9) . . ?
C6 N3 Cu1 114.0(8) . . ?
C1 N4 C5 121.8(10) . . ?
C1 N4 Cu1 124.8(8) . . ?
C5 N4 Cu1 113.4(7) . . ?
C11 N5 C15 120.1(10) . . ?
C11 N5 Cu2 125.9(8) . . ?
C15 N5 Cu2 114.0(8) . . ?
C20 N6 C16 121.2(10) . . ?
C20 N6 Cu2 115.4(8) . . ?
C16 N6 Cu2 123.4(9) . . ?
N4 C1 C2 120.2(13) . . ?
C3 C2 C1 119.3(15) . . ?
C2 C3 C4 119.6(14) . . ?
C3 C4 C5 119.1(15) . . ?
N4 C5 C4 119.9(12) . . ?
N4 C5 C6 116.1(9) . . ?
C4 C5 C6 123.9(12) . . ?
N3 C6 C7 121.1(13) . . ?
N3 C6 C5 113.8(9) . . ?
C7 C6 C5 125.2(12) . . ?
C8 C7 C6 119.3(15) . . ?
C7 C8 C9 119.8(13) . . ?
C8 C9 C10 120.5(15) . . ?
N3 C10 C9 117.6(15) . . ?
N5 C11 C12 120.6(13) . . ?
C13 C12 C11 118.8(15) . . ?
C12 C13 C14 121.3(13) . . ?
C15 C14 C13 116.9(14) . . ?
N5 C15 C14 122.3(13) . . ?
N5 C15 C20 114.8(10) . . ?
C14 C15 C20 122.9(12) . . ?
N6 C16 C17 120.1(14) . . ?
C18 C17 C16 117.7(16) . . ?
C17 C18 C19 122.7(14) . . ?
C20 C19 C18 116.1(15) . . ?
N6 C20 C19 122.2(13) . . ?
N6 C20 C15 113.5(9) . . ?
C19 C20 C15 124.2(13) . . ?
N2 C21 C22 120.8(11) . . ?
C21 C22 C23 118.6(12) . . ?
C24 C23 C22 118.6(10) . . ?
C25 C24 C23 119.8(10) . . ?
N2 C25 C24 121.2(11) . . ?
N2 C25 C26 114.4(9) . . ?
C24 C25 C26 124.3(10) . . ?
N1 C26 C27 121.6(11) . . ?
N1 C26 C25 114.8(9) . . ?
C27 C26 C25 123.5(10) . . ?
C26 C27 C28 117.9(10) . . ?
C29 C28 C27 120.0(11) . . ?
C28 C29 C30 118.8(12) . . ?
N1 C30 C29 121.8(11) . . ?

_refine_diff_density_max         1.996
_refine_diff_density_min         -1.533
_refine_diff_density_rms         0.267

